Mrs.S.A.Agrawal Int. Journal of Engineering Research and Application Vol. 3, Issue 5, Sep-Oct 2013, pp.261-265

RESEARCH ARTICLE

www.ijera.com

OPEN ACCESS

Study Of Height Dependency Of Drape Parameters. Mrs. S. A. Agrawal. Textile Engineering Department, Faculty of Technology and Engineering, the M S University of Baroda, Vadodara, India

Abstract:-Drape coefficient is a dependent value which itself is not sufficient to describe drape. Along, with this other drape parameters are also required to have a profound understanding of drape. In this paper it has been tried to find out the height dependency of these parameters to explain drape more explicitly. It shows that a positive correlation exists between the height of hanging and drape coefficient, Nodal length whereas a negative correlation exists with drape distance ratio. Poor correlation is seen with other parameters. These outcomes can be used to improve garment designing applications. Keywords: - Drape, Drape coefficient, Height of Hanging, Node parameters, Drape parameters

I.

INTRODUCTION

The role of drape in a garment is an important aspect of aesthetics. Drape can be defined as a property which characterizes the shape of a fabric when it is hanging down of its own weight. Drape is a unique property that allows a fabric to be bent in more than one direction describing a sense of graceful appearance. (11, 13) Drape properties are needed when modeling the cloth in virtual environment. (1, 6, 12) The drape coefficient is the widely used parameter to describe fabric drape but it needs other parameters to explain the fabric drape behavior. (2) Thus it may be better to use these parameters along with coefficient values as the latter is affected by the former. (3, 4). It has been explained earlier that for complete understanding of fabric drape profile node parameters such as number of nodes, nodal length, nodal distance and other drape parameters such as drape distance ratio, fold depth index and amplitude are required. (5, 7-9). The correlation between node parameters and constructional & bending properties has been studied (9). In the present study it has been tried to find out how the node parameter & drape parameter will be affected on changing the height of hanging of the fabric. By considering different heights a perspective of how a particular fabric which has been used to manufacture a garment appears on individuals of different heights can be studied. Here, the basic aim of this study is analyze the dependency of height on drape considering different drape parameters.

II.

given on the rod which is used to hold the supporting disc. The fabric sample was hang then height of hanging was considered from the point of hanging as in figure 1 Node parameters were calculated by using manual method where a centre was marked on the ammonia sheet and as the shadow is casted and cut, the node parameters such as no of nodes, nodal length and node distance are marked and measured. In earlier papers the measurement of these parameters was done according earlier discussed paper. (8-9) but here it is done manually as per figure 2. Also, other drape parameters like Drape Distance Ratio, Amplitude and Fold Depth Index were measured and calculated as depicted in figure 3. In the given figure and formulas ‘As’ is Area of draped fabric sample, ‘A1’ is Area of the fabric supporting disc, ‘A2’ is Area of the fabric sample disc,’ r1 ‘is radius of fabric supporting disc, ‘r2 ‘is radius of fabric sample disc,’ r min ‘is the minimum radius of the draped fabric sample,’ r max ‘is the maximum radius of the draped fabric sample (12) The formulas used are given as: Drape coefficient= [As-A1]/[A2-A1] Drape Distance Ratio= [(r2-ravg/ (r2-r1)]*100 Fold Depth Index = [(rmax-rmin/ (r2-r1)]*100 Amplitude = (rmax-rmin)/2 [12]

MATERIALS AND METHOD

Samples used are 100% cotton fabrics with warp and weft counts as 2/20s and 2/40s respectively. The structural parameters like end per inch, picks per inch, thickness & gsm were measured. For finding out the effect of height on these drape parameters different hanging height of the fabric were considered for each sample as per the table. The height can be changed with the help of marking www.ijera.com

261 | P a g e

Mrs.S.A.Agrawal Int. Journal of Engineering Research and Application Vol. 3, Issue 5, Sep-Oct 2013, pp.261-265

III.

www.ijera.com

RESULTS AND DISCUSSION

The structural parameters of given fabric samples were taken .The end/inch of fabric is kept constant whereas the picks/inch is varied from 3652.The fabric thickness range 0.046-0.053 cm. The fabric weight is 140-170 gsm. The seven drape parameters are being calculated and summarized in the table 1.The measurement taken on different height of hanging is being depicted. The correlation of these drape parameters with the height of hanging is shown in graphs (1-7). It is clear from the graphs (1, 2, 4) that as the height of hanging the fabric is increasing the drape coefficient and Nodal length shows an increasing trend whereas Drape distance ratio shows decreasing trend. No clear trend is observed Nodal distance, no of nodes ,FDI,Amplitude.Good correlation is found between the height of hanging and Drape parameters such as Drape coefficient (0.71), Nodal length (0.66). Negative correlation is found with drape distance ratio (-0.71). Poor correlation is found between the height of hanging and other drape parameters such as Nodal distance, No. of Nodes, Fold depth index & Amplitude. High correlation is also find between the parameters such as Nodal length & drape coefficient (0.714), Nodal distance (0.736).

Figure 1: Method for considering different heights.

Figure 2: Diagram depicting manual method of calculating node parameters. (N.L-Nodal length, N.D-Nodal distance

Figure 3: Diagram depicting different measures for calculation of drape

Parameters. Graph 1: Correlation between Height of Hanging and drape coefficient Drape coefficient

80.00 S1

60.00

S2 40.00

S3

20.00

S4 S5

0.00 6.4

www.ijera.com

6.6

6.8

Height 7 of hanging 7.2

7.4

7.6

7.8

262 | P a g e

Mrs.S.A.Agrawal Int. Journal of Engineering Research and Application Vol. 3, Issue 5, Sep-Oct 2013, pp.261-265

www.ijera.com

Table: Drape parameters for the analyzed fabrics Sample

Drape Parameters

Height(cms) 6.5

S1

Drape coefficient No of Nodes Nodal length(cm) Nodal distance(cm) Drape distance ratio Fold depth Index Amplitude(cm) Drape coefficient No of Nodes Nodal length(cm) Nodal distance(cm) Drape distance ratio Fold depth Index Amplitude(cm) Drape coefficient No of Nodes Nodal length(cm) Nodal distance(cm) Drape distance ratio Fold depth Index Amplitude(cm) Drape coefficient No of Nodes Nodal length(cm) Nodal distance(cm) Drape distance ratio Fold depth Index Amplitude(cm) Drape coefficient No of Nodes Nodal length(cm) Nodal distance(cm) Drape distance ratio Fold depth Index Amplitude(cm)

S2

S3

S4

S5

58.34 5 12.3 11.5 0.341 14.4 0.45 59.47 5 12.4 12.4 0.331 35.2 1.1 66.64 5 12.4 14.8 0.268 91.2 2.85 59.85 4 12.6 14.5 0.328 24 0.75 63.62 5 12.5 11.7 0.294 46.4 1.45

6.8 59.47 5 12.4 14.9 0.331 20.8 0.65 63.62 5 12.8 17.9 0.294 28.8 0.9 67.40 4 12.9 15.1 0.261 24 0.75 68.53 5 12.8 15.1 0.251 59.2 1.85 68.15 6 12.7 14.8 0.255 94.4 2.95

7.1 66.64 4 12.5 16.4 0.268 25.6 0.8 73.06 5 12.8 14.6 0.213 25.6 0.8 70.41 4 13.3 18.3 0.235 12.8 0.4 69.28 5 12.8 14.8 0.245 24 0.75 74.19 5 12.7 14.6 0.204 30.4 0.95

7.4 67.02 5 12.7 14.9 0.264 64 2 74.19 4 12.9 15 0.204 22.4 0.7 71.55 5 13.4 17.4 0.226 24 0.75 70.79 5 13.1 15.3 0.232 59.2 1.85 74.56 5 13.1 14.7 0.200 19.2 0.6

7.7 68.15 5 12.8 14.5 0.255 28.8 0.9 75.32 6 13.1 15.3 0.194 32 1 75.70 5 13.1 15.2 0.191 24 0.75 74.94 5 13.9 19.6 0.197 3.2 0.1 75.32 6 12.8 15.1 0.194 32 1

Graph 2: Correlation between Height of Hanging and Nodal length Nodal Length

14.00 S1

13.50

S2 13.00

S3 S4

12.50

S5 12.00 6.4

www.ijera.com

6.6

6.8

Height 7 of Hanging 7.2

7.4

7.6

7.8

263 | P a g e

www.ijera.com

Graph 3: Correlation between Height of Hanging and Nodal distance Nodal distance

25.00 20.00

S1

15.00

S2

10.00

S3

5.00

S4 S5

0.00 6.4

6.6

6.8

Height 7 of hanging 7.2

7.4

7.6

7.8

Graph 4: Correlation between Height of Hanging and No. of Nodes No. Of Nodes

8 S1

6

S2 4

S3

2

S4 S5

0 6.4

6.6

6.8

Height 7 of Hanging 7.2

7.4

7.6

7.8

Graph 5: Correlation between Height of Hanging and drape distance ratio Drape distance ratio

40.00 S1

30.00

S2

20.00

S3

10.00

S4

0.00

S5 6.4

6.6

6.8

Height 7 of hanging 7.2

7.4

7.6

7.8

Graph 6: Correlation between Height of Hanging and Fold Depth Index Fold Depth index

100 80

S1

60

S2

40

S3 S4

20

S5

0 6.4

6.6

6.8

Height 7 of Hanging 7.2

7.4

7.6

7.8

Graph 7: Correlation between Height of Hanging and Amplitude

Amplitude

4 S1

3

S2 2

S3

1

S4

0

S5 6.4

6.6

IV.

6.8

7 7.2 Height of Hanging

CONCLUSION

In this study, the various drape parameters of woven fabrics were measured. The seven drape parameters such as drape coefficient (DC), Nodal length (NL), Nodal Distance (ND), drape distance ratio (DDR), fold depth index (FDI), amplitude (A) and number of nodes (N) were measured by using the www.ijera.com

7.4

7.6

7.8

ammonia paper sheet. These parameters help to understand the drapability of fabric in terms of its shape. Also, the height dependency of these parameters was studied by taking different hanging heights and analyzes of its effect on these parameters was done. There is a strong correlation between height of hanging and drape coefficient, Nodal length 264 | P a g e

Mrs.S.A.Agrawal Int. Journal of Engineering Research and Application Vol. 3, Issue 5, Sep-Oct 2013, pp.261-265 whereas Negative correlation is observed with drape distance ratio.It enables to understand how the same fabric exhibits different draping behavior at different heights and hence would behave differently as garments on individual of variable heights. It can be helpful for getting a perspective of how the fabric looks when same garment design is manufactured for different height individuals.

REFERENCE [1]

[2]

[3]

[4]

[5]

[6] [7]

[8]

[9]

[10]

[11]

Mailis Mäkinen and Harriet Meinander, “Influence of Physical Parameters on abric Hand”,Tampere University of Technology, SmartWearLab, Christiane Luible and Nadia Magnenat-Thalmann University of Geneva, MIRALab. Ajit Kumar Pattanayak, Ameersing Luximon and Asimananda Khandual,” Prediction of drape profile of cotton woven fabrics using artificial neural network and multiple regression method”, Textile Research Journal 81(6) 559–566. Stylos GK and Wan TR. The concept of virtual measurement – 3D fabric drapability. Int J Cloth Sci Tech 1999; 11(1): 10–18. Matsudaira M and Zhang YM. Method of measuring drape coefficient of fabrics and the regression equation with mechanical parameters. Proceedings 26th Textile Research Symposium Mt. Fuji, Fibrous Materials Research Group Kyoto. 1997, pp.219–224. Behera BK and Pangadiya A. Drape measurement by digital image processing. Textile Asia 2003; 34(11): 45–50. Saville BP ‘Physical testing of textiles’. Cambridge: Woodhead.2000.p.310. G.Thilagavathi and V.Natarajan,”Development of a method for measurement of fabric three Dimensional drape and studies on influencing factors, IFJTR, 2003, pp 41-49 S.A.Agrawal & D.A.Vasavda,”Three Dimensional Measurement of Drape”, Journal of the Textile Association, Nov-Dec 2009, pp 155-162. S.A.Agrawal,” Node Parameters and Its Relation with Constructional and Bending Properties of PC Blended Fabric”, International Journal of Engineering Research and Development, Volume 5, Issue 7 (January 2012), PP. 61-66 Ajit Kumar Pattanayak, Ameersing Luximon and Asimananda Khandual,” Prediction of drape profile of cotton woven fabrics using artificial neural network and multiple regression method”, Textile Research Journal ,81(6), 559–566 Ashok A Itagi, Arindam Basu,”Drape Behaviour of Silk Apparel Fabrics with

www.ijera.com

[12]

[13] [14]

www.ijera.com

Radial Seams”,International Journal of Engineering Research and Technology”,Vol.1,Issue-8,Oct 2012. B.K.Behera, Ajit Kumar Pattanayak,”Measuring and modeling of drape using digital image processing”,International Journal of Fibre Research & Textile Research”Vol 33,Oct 2008, PP 230-238. J.E.Booth,”Principle of Textile Testing”,London Heywood Books. S.A.Agrawal &et al,”Numerical Simulation of Three Dimensional Drape”,Man-made Textiles in India,October2011,pp 363-366.

265 | P a g e